First heterometallic Ga(III)-Dy(III) single-molecule magnets: implication of Ga(III) in extracting Fe-Dy interaction.
Chen, Sihuai; Mereacre, Valeriu; Anson, Christopher E.; Powell, Annie K.; Dalton transactions (Cambridge, England : 2003) 45 (2016) 9336–9344; doi:10.1039/c6dt01364c

data_7039238
_publ_section_title
;
 First heterometallic Ga(III)-Dy(III) single-molecule magnets: implication
 of Ga(III) in extracting Fe-Dy interaction.
;
_journal_issue                   22
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9336
_journal_page_last               9344
_journal_paper_doi               10.1039/c6dt01364c
_journal_volume                  45
_journal_year                    2016
_chemical_formula_moiety         'C128 H154 Dy4 Ga4 N4 O36, 4(C2 H3 N)'
_chemical_formula_sum            'C136 H168 Dy4 Ga4 N8 O36'
_chemical_formula_weight         3419.65
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     'dual-space direct methods'
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2016-03-08 deposited with the CCDC.
2016-05-09 downloaded from the CCDC.
;
_cell_angle_alpha                87.415(2)
_cell_angle_beta                 87.793(2)
_cell_angle_gamma                68.609(3)
_cell_formula_units_Z            2
_cell_length_a                   15.4662(4)
_cell_length_b                   16.8729(5)
_cell_length_c                   29.1650(8)
_cell_measurement_reflns_used    16347
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      28.71
_cell_measurement_theta_min      2.42
_cell_volume                     7077.4(4)
_computing_cell_refinement
;
CrysAlisPro 1.171.37.34 (Agilent Technologies, 2014)
;
_computing_data_collection
;
CrysAlisPro 1.171.37.34 (Agilent Technologies, 2014)
;
_computing_data_reduction
;
CrysAlisPro 1.171.37.34 (Agilent Technologies, 2014)
;
_computing_molecular_graphics    'Diamond 2.1 (Crystal Impact, 1998)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2015)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector_area_resol_mean 8.0534
_diffrn_detector_type            'Eos CCD'
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.961
_diffrn_measurement_device       'four-circle kappa-geometry diffractometer'
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Eos'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0454
_diffrn_reflns_av_unetI/netI     0.0859
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.961
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       36
_diffrn_reflns_limit_l_min       -36
_diffrn_reflns_number            60399
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.961
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.483
_diffrn_reflns_theta_min         2.240
_diffrn_source                   'SuperNova (Mo) Microfocus Source'
_exptl_absorpt_coefficient_mu    2.911
_exptl_absorpt_correction_T_max  0.892
_exptl_absorpt_correction_T_min  0.754
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.37.34 (Agilent Technologies, 2014)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.605
_exptl_crystal_description       block
_exptl_crystal_F_000             3432
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.050
_exptl_crystal_size_min          0.040
_refine_diff_density_max         1.892
_refine_diff_density_min         -4.036
_refine_diff_density_rms         0.167
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.122
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1704
_refine_ls_number_reflns         31158
_refine_ls_number_restraints     51
_refine_ls_restrained_S_all      1.124
_refine_ls_R_factor_all          0.0976
_refine_ls_R_factor_gt           0.0653
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0115P)^2^+41.7345P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1062
_refine_ls_wR_factor_ref         0.1196
_reflns_Friedel_coverage         0.000
_reflns_number_gt                22467
_reflns_number_total             31158
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6dt01364c2.cif
_cod_data_source_block           1444Ga
_cod_depositor_comments
'Adding full bibliography for 7039237--7039238.cif.'
_cod_database_code               7039238
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.780
_shelx_estimated_absorpt_t_max   0.892
_shelx_res_checksum              66080